International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
STUDY OF CELLULAR STRUCTURES: ANALYSIS OF ELASTIC DEFORMATION OF ALUMINIUM HONEYCOMBS Sprika Gaur, Rashmi Rama Sushil, Rakesh Saxena1 1Department
of Mechanical Engineering, G. B. Pant University of Agriculture and Technology, Pantnagar, India ***The most important feature of a cellular solid is its relative ABSTRACT  Cellular solids are an assembly of a number of cells forming solid edges or faces and occupying space. Honeycombs are a twodimensional array of such cells, forming polygons for faces. It exists in nature as wood, coral etc. They are also manufactured and used widely as polymeric foams. A background study of honeycomb history has been conducted from Gibson and Ashby’s model, which describes a relationship between the Young’s Modulus of a regular hexagonal honeycomb cell and that of the material from which the honeycomb cell has been made, to Balawi and Abot’s model of commercial honeycombs with double cell wall thickness. This work investigates the inplane elastic properties of regular aluminium honeycomb cells of t/l ratios 0.3 and 0.005 using ANSYS Mechanical. Software implications have been used to carry out comparisons between the trends of elastic deformation, normal vs shear stress and maximum principal stress vs maximum principal elastic strain of honeycomb cells as a whole and of the outer slant edge of the cell. Inplane elastic properties of commercial honeycomb cell of t/l ratio 0.005 have, also, been compared with the regular honeycomb cell of the same ratio.
density, that is, the ratio of the density of the cellular solid and that of the solid from which the cells are made. As this density ratio increases, the pore spaces shrink and the cell wall thickens. Above a relative density of about 0.3, there is a transition from cellular solids to solid structure merely containing pores. Therefore, true cellular solids are considered to have a relative density of less than 0.3.
Keywords: Cellular Solids, Honeycombs, Inplane elastic properties, Commercial Honeycombs, Shear stress, Normal stress, Maximum Principal Stress, Maximum Principal Elastic Strain
The physical, thermal and chemical properties of cellular solids can be measured in the same way as that of true solids. Foaming in various materials expanses the scope of usage of that material. It creates an extension of properties, paving way for more advanced engineering applications, which otherwise would not have been possible without it. On the basis of the distribution of solid in cells and edges, the properties of cellular solids may vary. Hence, quantifying the structure, to understand the various properties of cellular solids has to be the initial step. Geometrical aspects of cell structure such as relative density and anisotropy and topological aspects of cell shape such as number of neighbouring contacts and edge and face connectivity are also pivotal to understanding the mechanical properties of cellular structures.
1. INTRODUCTION Cellular solids are an assembly of a number of cells forming solid edges or faces and occupying space. Honeycombs are a twodimensional array of such cells, forming polygons for faces. The term ‘honeycomb’ represents all 2D cellular solid forming polygons. Foams are a threedimensional array of cells, which occupy space. The cells, here, form polyhedral solids, which are solids made up of plane surfaces. Foams are of two types, open celled foams and closed celled foams. If the cells of a solid are connected by open surfaces only, then it is called an open celled foam. On the other hand, if the cells of a solid are completely separated out from the neighbouring cells by solid faces, then it is called a closed celled foam.
© 2019, IRJET

Impact Factor value: 7.34

The objective of this research article is to develop ANSYS models of two aluminium honeycombs of t/l ratios 0.005 and 0.3 and analyse and compare their inplane elastic properties, in terms of deformation, normal stress, shear stress, maximum principal stress and maximum principal elastic strain, under uniaxial compressive loading in the two inplane directions, namely X and Y, and to study the elastic inplane deformation of commercial honeycombs of t/l ratio 0.005 under uniaxial compressive loading. These ratios are taken so that the properties of true cellular solids can be compared with solid structures containing pores.
2. PROPERTIES
3. APPLICATIONS Cellular solids are manufactured and used widely as polymeric foams, which are used in everything from crash
ISO 9001:2008 Certified Journal

Page 1583
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
padding of an aeroplane to disposable cups. It is now easier to foam not only polymers, but also metals used for cushioning and insulation. The deHavilland Mosquito aircraft (a WWII bomber) is considered to be the ﬁrst industrial scale application of honeycombs. Commercially available honeycombs usually have low relative density [1]. Polymeric and glass foams are used for thermal insulation of booster rockets for space shuttle, refrigerated trucks, railway cars and ships carrying liquid natural gas. They are also used in skis, racing yachts and portable buildings. The cuttlebone in cuttlefish is an example of an elaborate sandwich panel. The skull is made up of two layers of dense bones separated by a lightweight spongy core of cancellous bone. They are extensively used as flotation in boats and as supports for floating structures. Foams and honeycombs have special advantages as filters, carriers for inks and dyes, waterrepellent membranes etc.
4. BACKGROUND As mentioned before, the deHavilland Mosquito aircraft (a WWII bomber) is considered to be the ﬁrst industrial scale application of honeycombs (Tom, 1997[3]; Hoffman, 1958[4]). In the beginning, honeycombs were used as sandwich structures for high outofplane stiffness and as lowdensity impact energy absorption materials (Zhao and Grrard, 1998[5]; Vinson, 1999[6]; Khan, 2006[7]). Olympio and Gandhi in 2007[8], Bubert et al. in 2008[9] and Jaehyung et al. in 2010[10] proposed high shear strength and strain honeycomb structures. Kwangwon Kim et al., in 2012 [11] proposed FEA models of modified Auxetic honeycombs, honeycombs with negative Poisson’s ratio, as high strain flexures. Yanping and Hong [12] in 2010 gave a detailed review of Auxetic cellular structures. Garrard (1949) [13], Charles and Ralph (1951) [14] and Horvay (1952) [15] studied the overall elastic properties of sandwich plates in the assembled situation. While Akasaka and Takagishi (1959) [16], Hoffman (1958) and Kelsey et al. (1958) [17] studied the inplane Poisson’s ratio of hexagonal honeycomb cores and the effective transverse shear moduli. Habip (1964) [18], Lui and Habip (1965) [19] worked towards attaining efficiency in numerical analysis. (Frostig, 1998) [20] showed that for this, by application of a composite or sandwich shell theory, a continuum model replaces the honeycomb core and analysed in terms of their eﬀective properties. Cell geometries were also proposed by many such as, Theocaris et al. (1997) [21] (starshaped microstructure), Grima et al. (2008b) [22] (Chiral honeycombs), Larsen et al. (1997) [23], Smith et al. (2000) [24] , Gaspar et al. (2005),
© 2019, IRJET

Impact Factor value: 7.34

Kwangwon Kim et al. (2012) [25] and Jaehyung et al. (2010) [26] ,but were later proved to have no practical purposes. Lorna Gibson and Michael Ashby (1988) [27] considered the honeycomb cell walls to be flexures that is fixed at one end and guided at the other end, using the Cellular Material Theory, which is a cell wall bending model. Later on, Masters and Evans (1996) [28] modified the model by introducing three mechanisms of flexing, hinging and stretching. Hohe and Becker (2002) [29] presented a thorough examination of the homogenization methods and material models. Balawi and Abot (2007b) [30] and Balawi and Abot (2008) [31] proposed a model for commercial honeycombs, which are honeycombs with double cell wall thickness in the vertical direction.
5. MECHANICS OF HONEYCOMBS When a honeycomb is compressed inplane, the cells walls will first bend giving linear deformation. After the critical value of the strain is reached, the cells collapse by elastic buckling, plastic yielding, brittle fracture or creep, depending upon the nature of the cell wall material. Furthermore, as the collapse continues and the opposing cell walls begin to touch each other, and the collapse ends densifying the structure and increasing the stiffness rapidly. Elastomeric materials collapse by elastic buckling. This collapse is recoverable. In brittle materials, the collapse is by brittle fracture of cell wall. While in materials with plastic yield point, the deformation is by formation of plastic hinges at the section of maximum moment in the bent cell walls. The collapse is irrecoverable in both of these cases.
Image 1: The inplane and outofplane directions of a honeycomb which are X and Y, and Z respectively. The inplane stresses and strengths are lower as compared to the outofplane stresses and strengths because loading in the former directions make the cell walls bend. Study of inplane properties shows the mechanism by which cellular solids deform and fail, while the study of outofplane properties gives us the details of the additional stiffness, which is primary in understanding the behaviour of natural honeycomblike materials, such as wood. A regular hexagonal honeycomb with uniform cell wall thickness is isotropic. Such a structure has two
ISO 9001:2008 Certified Journal

Page 1584
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
independent elastic moduli, a Young’s modulus E* and a shear modulus G*, for instance, and a single value of plateau stress σ*. The three main assumptions which make the study of the inplane properties of honeycombs easier, as described by the Gibson and Ashby’s model, are: 1. 2. 3.
The cell walls are linearly elastic and isotropic. The deformations are small and, hence, small changes in geometry can be neglected. The t/l ratio or the relative density is small and therefore, shear and axial contributions to the deformation can be neglected.
Gibson and Ashby carried out the analysis for the inplane properties of a hexagonal honeycomb assuming that the inclined walls of a unit cell will deflect as a beam resulting in a dependence on the cubic wall thickness to wall length ratio, (t/l)3. Furthermore, the deflection from axial deformation of the vertical walls is much lower than the deflection due to bending of the inclined wall, so it can be neglected for lower values of t/l. Masters and Evans modified the models presented by Gibson and Ashby by introducing the hinging of the walls at the intersection points of the inclined and vertical cell walls, which resulted in the dependence on the t/l ratio, resulting in lower effects on the overall inplane properties of the honeycomb. Commercial honeycombs have double cell wall thickness in the vertical direction. This double wall occurs as a result of most common production methods such as expansion and sheet corrugation [37]. The analysis of the inplane properties neglects the vertical wall deformation, therefore, both regular honeycombs with uniform thickness and double cell wall thickness in the vertical direction will have the same inplane properties. Although, a thorough examination of this assumption shows that this cannot be the case. Experimental results show that for honeycombs with higher relative density, there is a difference between the elastic moduli where E 2eff is higher than that calculated for E1eff (Balawi and Abot, 2007), although this difference is not very significant in commercial honeycombs. This may be due to the difference in the hole shapes during machining, faulty manufacturing processes, and the stress relieving process experienced by the studied honeycomb.
direction in ANSYS Workbench (Static Structural). In both the cells, l= 10 mm, and t= 0.05 mm and t= 3 mm for cells of t/l ratio 0.005 and 0.3 respectively. The former unit cell denotes a cellular solid which conforms to the relative density requirements of an optimum cellular solid. We already know that cellular solids with relative density ratios greater than 0.3 are simply considered to be solid structures with holes in them. Therefore, for comparison, a unit cell of t/l ratio 0.3 is taken into consideration. It is important to note here that the relative density ratio of a hexagonal honeycomb is directly proportion to the t/l ratio, hence, their uses in the text are somewhat similar. Both the unit cells created also have the connecting edges of the adjacent cells up to a length of 0.4 mm. For calculations the entire cells and the outer slant edges are considered. The reason for choosing the latter is that its deformation is also affected by that of the vertical edge connected to it. S. No. 1 2
3 4 5 6
Property Density Isotropic Elasticity (Derive From) Young’s Modulus Poisson’s Ratio Bulk Modulus Shear Modulus Tensile Yield Strength Compressive Yield Strength Tensile Ultimate Strength Compressive Ultimate Strength
Value 2770
Unit Kg m3
7.1E+10 0.33 6.9608E+10 2.6692E+10 2.8E+08
Pa
2.8E+08
Pa
3.1E+08
Pa
0
Pa
Table 1: Properties of Aluminium alloy used to create the honeycomb cells.
Image 3: Compressive deformation of value 0.001 m applied on the negative and positive X directions.
6. SPECIFICATIONS AND DESIGN Two planar surfaces of aluminium hexagonal unit cells with t/l ratios 0.005 and 0.3 were modelled in SOLIDWORKS and were given a thickness of 0.001 m in Z
© 2019, IRJET

Impact Factor value: 7.34

Pa Pa Pa
ISO 9001:2008 Certified Journal

Page 1585
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
The value of deformation in X direction for both the cells is negative. Also, the cell with t/l ratio 0.005, starts its deformation at a higher value than the other cell. But, eventually, at the end of the time period of 1 second, the value of deformation converges to a somewhat similar value for both the cells.
7. RESULTS AND DISCUSSIONS A compressive deformation of 0.001 m is applied in the positive and negative X directions and the total deformation, deformation in X direction and deformation in Y direction of the outer slant edge of regular hexagonal cells of t/l ratios 0.3 and 0.005 are calculated. The total deformation for both the cells is positive and converges to a common value once. The cell with t/l ratio 0.005 deforms more as it starts its deformation at a closer value to the given deformation of 0.001 m and the calculated value at the end of 1 second is also lower for this cell, meaning that the stretch of deformation for this cell is more.
Chart 1: Total deformation in m of the outer slant edge of hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative X directions in 1 second.
ÂŠ 2019, IRJET

Impact Factor value: 7.34

Deformation in X direction in m
Image 5: Outer slant edge in the cell.
t/l= 0.3 t/l= 0.005 0 1
2
3
4
5
6
7
8
9
10
0.0001 0.0002 0.0003 0.0004 0.0005 0.0006
No. of Divisions of 1 second Chart 2: Deformation in X direction in m of the outer slant edge of hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative X directions in 1 second. The value of deformation in the Y direction for both the cells is negative and starts at values very close to each other. At the end of 1 second, the cell with t/l ratio 0.005 has a much bigger deformation stretch than the cell with t/l ratio 0.3.
Deformation in Y direction in m
Image 4: Compressive deformation of value 0.001 m applied on the positive and negative Y directions.
0 0.0001 0.0002 0.0003 0.0004 0.0005 0.0006 0.0007 0.0008 0.0009 0.001
t/l= 0.3 t/l= 0.005 1
2
3
4
5
6
7
8
9
10
No. of divisions of 1 second
Chart 3: Deformation in Y direction in m of the outer slant edge of hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative X directions in 1 second.
ISO 9001:2008 Certified Journal

Page 1586
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
Total Deformation in m
The values of total deformation in both the cells is positive and follows a somewhat same trend. t/l= 0.3 t/l= 0.005
0.0012 0.001 0.0008 0.0006
The values of deformation in the Y direction for both the cells are positive and follows a somewhat similar trend. t/l= 0.3 t/l= 0.005
Deformation in Y direction in m
A compressive deformation of 0.001 m is applied in the positive and negative Y directions and the total deformation, deformation in X direction and deformation in Y direction of the outer slant edge of regular hexagonal cells of t/l ratios 0.3 and 0.005 are calculated.
0.0012 0.001 0.0008 0.0006 0.0004 0.0002 0 1
2
0.0004
0 2
3
4
5
6
7
8
9
4
5
6
7
8
9
10
Chart 6: Deformation in Y direction in m of the outer slant edge of hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative Y directions in 1 second.
0.0002 1
3
No. of divisions of 1 second
10
No. of divisions of 1 second Chart 4: Total deformation in m of the outer slant edge of hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative Y directions in 1 second.
A compressive deformation of 0.001 m is applied in the positive and negative X directions and the total deformation, deformation in X direction and deformation in Y direction of the entire regular hexagonal cells of t/l ratios 0.3 and 0.005 are calculated.
The values of deformation in X direction for both the cells start at a positive value and then reduces to a negative value. The cell with the t/l ratio 0.005 has a much lower value of deformation at the end of 1 second as compared to the cell with t/l ratio 0.3.
The values of total deformation in both the cells are positive and follow a somewhat similar trend. Also, at the end of 1 second, both the deformation values converge to zero.
0.00005 0 0.00005
1
2
3
4
5
6
7
8
9 10
0.0001 0.00015 0.0002 0.00025 0.0003
0.001 0.0008 0.0006 0.0004 0.0002 0
0.00035
1
No. of divisions of 1 second
Chart 5: Deformation in X direction in m of the outer slant edge of hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative Y directions in 1 second.
ÂŠ 2019, IRJET
t/l= 0.3 t/l= 0.005
0.0012
Total Deformation in m
Deformation in X direction in m
t/l= 0.3 t/l= 0.005

Impact Factor value: 7.34

2
3
4
5
6
7
8
9
10
No. of divisions od 1 second Chart 7: Total deformation in m of the entire hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative X directions in 1 second.
ISO 9001:2008 Certified Journal

Page 1587
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
The values of deformation in the X direction for both the cells start at a positive value and at the end of 1 second, becomes negative, while following a similar trend. t/l= 0.3 0.0002
t/l= 0.3 t/l= 0.005
0 2
3
4
5
6
7
8
9
10 0.0012
0.0004 0.0006 0.0008 0.001 0.0012
No. of divisions of 1 second
The values of deformation in the Y direction for both the cells start at a positive value and ends at a negative value. The stretch of deformation values is more for the cell with t/l ratio 0.005 as compared to the other cell. In the graph, it is observable that the values of deformation for both the cells will have a similar value. t/l= 0.3 t/l= 0.005 0.001 0.0008 0.0006 0.0004 0.0002 0 0.0002 0.0004 0.0006 0.0008 0.001
Total Deformation in m
0.0002
1
Chart 8: Deformation in X direction in m of the entire hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative X directions in 1 second.
Deformation in Y direction in m
The values of total deformation in both the cells is positive and follows a similar trend. At the end of 1 second, the deformation values end at zero.
0.001 0.0008 0.0006 0.0004 0.0002 0 1
2
3
4
5
6
7
8
9
10
No. of divisions of 1 second Chart 10: Total deformation in m of the entire hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative Y directions in 1 second. The values of deformation in X direction of both the cells start at a positive value and at the end of the 1 second becomes negative in value. Both the cells follow a similar trend in the deformation and have values very close to each other. t/l= 0.3 t/l= 0.005
1
2
3
4
5
6
7
8
9
10
No. of divisions of 1 second
Chart 9: Deformation in Y direction in m of the entire hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative X directions in 1 second. A compressive deformation of 0.001 m is applied in the positive and negative Y directions and the total deformation, deformation in X direction and deformation
ÂŠ 2019, IRJET

Impact Factor value: 7.34

Deformation in X direction in m
Deformation in X direction in m
t/l= 0.005
in Y direction of the entire regular hexagonal cells of t/l ratios 0.3 and 0.005 are calculated.
0.0005 0.0004 0.0003 0.0002 0.0001 0 0.0001 0.0002 0.0003 0.0004 0.0005
1
2
3
4
5
6
7
8
9
10
No. of divisions of 1 second
Chart 11: Deformation in X direction in m of the entire hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative Y directions in 1 second.
ISO 9001:2008 Certified Journal

Page 1588
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
The values of deformation in Y direction for both the cells are positive with the values approaching zero at the end of one second. Both the cells follow a similar trend with values very close to each other. t/l= 0.3
0.001 0.0008 0.0006
y = 7E+10x  471630
100000000 80000000 60000000 40000000 20000000 0 0
0.0005
0.001
0.0015
0.002
Chart 13: Maximum Principal Elastic Strain vs Maximum Principal Stress in Pa for cell of t/l ratio 0.005 when a compressive deformation of 0.001 m is applied in the positive and negative X directions.
0.0002 0
0.0002
120000000
Maximum Principal Elastic Strain in Pa
0.0004
1
2
3
4
5
6
7
8
9
10
No. of divisions of 1 seocnd
Chart 12: Deformation in Y direction in m of the entire hexagonal cells of t/l ratios 0.3 and 0.005 when a deformation of 0.001 m is applied in positive and negative Y directions in 1 second. A compressive deformation of 0.001 m is applied in the positive and negative X directions and an evaluation of the Maximum Principal Elastic Strain and Maximum Principal Stress is done on the entire cells of t/l ratios 0.005 and 0.3. In both the cells, the graphs constitute of ten values of stress and strain calculated in ten divisions of one second. The values of stress and strain, for both the cells, decreases with our calculation time and the graph gives us a straightline trend between stress and strain. The maximum of stress and strain for the latter cell are, approximately, 14.56 times and 15.85 times of that of the former cell, respectively. While the minimum values of stress and strain for the latter cell are, approximately 14.54 and 16.68 times of that of the former cell, respectively.
Maximum Principal Stress in Pa
Deformation in Y direction in m
t/l= 0.005 0.0012
Maximum Principal Stress in Pa
www.irjet.net
120000000 y = 7E+10x  471630
100000000 80000000 60000000 40000000 20000000 0 0
0.0005
0.001
0.0015
0.002
Maximum Principal Elastic Strain in Pa Chart 14: Maximum Principal Elastic Strain vs Maximum Principal Stress in Pa for cell of t/l ratio 0.3 when a compressive deformation of 0.001 m is applied in the positive and negative X directions. A compressive deformation of 0.001 m is applied in the positive and negative Y directions and an evaluation of the Maximum Principal Elastic Strain and Maximum Principal Stress is done on the entire cells of t/l ratios 0.005 and 0.3. The values of stress and strain, for both cells, decreases and the graph gives us a straightline trend between stress and strain. The maximum value of stress and strain for the latter are, approximately, 31.67 times and 31.89 times that of the former cell, respectively. While the minimum values of stress and strain for the latter cell are, approximately, 31.74 times and 32.14 times that of the former cell, respectively.
ÂŠ 2019, IRJET

Impact Factor value: 7.34

ISO 9001:2008 Certified Journal

Page 1589
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
120000000
Normal Stress in X direction Shear Stress in XY plane
y = 7E+10x  471630
100000000
1.50E+09
80000000
1.00E+09
60000000
5.00E+08
Stress in Pa
Maximum Principal Stress in Pa
International Research Journal of Engineering and Technology (IRJET)
40000000 20000000 0 0
0.0005
0.001
0.0015
0.00E+00 5.00E+08
1
2
5
6
7
8
9
10
1.00E+09 1.50E+09 2.50E+09 3.00E+09
Chart 15: Maximum Principal Elastic Strain vs Maximum Principal Stress in Pa for cell of t/l ratio 0.005 when a compressive deformation of 0.001 m is applied in the positive and negative Y directions.
Maximum Principal Stress in Pa
4
2.00E+09
0.002
Maximum Principal Elastic Strain in Pa
120000000
No. of divisions of 1 second
Chart 17: Normal stress in X direction and Shear stress in XY plane in Pa for the entire hexagonal cell of t/l ratio 0.3 when a compressive deformation of 0.001 m is applied in the positive and negative X directions. When the outer slant edge is evaluated, it is found that both the stress values start at some positive values, with the normal stress being greater than the shear stress by 1.4 times. But, as the deformation progresses, the values of stresses become negative and at the end of one second, the value of shear stress becomes 1.4 times greater than that of the normal stress.
y = 7E+10x  471630
100000000
3
80000000 60000000 40000000 20000000
Normal Stress in X direction 0 0
0.0005
0.001
0.0015
Shear Stress in XY plane
0.002 1E+09
Maximum Principal Elastic Strain in Pa
A compressive deformation of 0.001 m is applied in the positive and negative X directions and an evaluation of the Normal Stress in X direction and of Shear Stress in XY plane is done on the entire cell and on the outer slant edge of the cell of t/l ratio 0.3. When the entire cell is evaluated, it is found that the maximum values of both the stresses is somewhat similar but after the end of one second, the shear stress is greater than the normal stress by 2.7 times.
500000000
Stress in Pa
Chart 16: Maximum Principal Elastic Strain vs Maximum Principal Stress in Pa for cell of t/l ratio 0.3 when a compressive deformation of 0.001 m is applied in the positive and negative Y directions.
0 1
2
3
4
5
6
7
8
9 10
5E+08 1E+09 1.5E+09
No. of divisions of 1 second
Chart 18: Normal stress in X direction and Shear stress in XY plane in Pa for the outer slant edge of the hexagonal cell of t/l ratio 0.3 when a compressive deformation of 0.001 m is applied in the positive and negative X directions. A compressive deformation of 0.001 m is applied in the positive and negative Y directions and an evaluation of the Normal Stress in X direction and of Shear Stress in XY plane is done on the entire cell and on the outer slant edge
ÂŠ 2019, IRJET

Impact Factor value: 7.34

ISO 9001:2008 Certified Journal

Page 1590
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
of a cell of t/l ratio 0.3. When the entire cell is evaluated, it is observed that the both the stress values start at a positive value and then later, become negative. The maximum value of normal stress is, approximately, 1.9 times that of the shear stress, while the minimum value of normal stress is, approximately, 1.23 times less than that of the shear stress.
A compressive deformation of 0.001 m is applied in the positive and negative X directions and an evaluation of the Normal Stress in X direction and of Shear Stress in XY plane is done on the entire cell and on the outer slant edge of a cell of t/l ratio 0.005. When the entire cell is evaluated, it is found that the maximum value of normal stress is, approximately, 1.7 times greater than that of the shear stress, while the minimum value of normal stress is, approximately, 1.7 times less than that of the shear stress at the end of 1 second. Normal Stress in Y direction Shear Stress in XY plane 40000000
Stress in Pa
20000000 0 1
2
3
4
5
6
7
8
9
10
20000000 40000000
19: Normal stress in X direction and Shear stress in XY plane in Pa for the entire hexagonal cell of t/l ratio 0.3 when a compressive deformation of 0.001 m is applied in the positive and negative Y directions.
No. of divisions of 1 second Chart 21: Normal stress in X direction and Shear stress in XY plane in Pa for the entire hexagonal cell of t/l ratio 0.005 when a compressive deformation of 0.001 m is applied in the positive and negative X directions.
When the outer slant edge is evaluated, it is found that the values of both the stresses start at positive, with the maximum shear stress being greater than the maximum normal stress by 2.7 times, and then move onto the negative value, with the minimum value of shear stress being greater than that of the normal stress by 7.26 times.
When the outer slant edge is evaluated, it is found that the maximum values of the two stress is somewhat same, while the minimum value of normal stress is 3.6 times less than that of the shear stress. Normal Stress in Y direction
20000000
1
2
3
4
5
6
7
8
9
10
10000000 0 10000000
1
2
3
4
5
6
7
8
9 10 11
20000000 30000000 40000000
No. of divisions on 1 second Chart 20: Normal stress in X direction and Shear stress in XY plane in Pa for the outer slant edge of the hexagonal cell of t/l ratio 0.3 when a compressive deformation of 0.001 m is applied in the positive and negative Y directions.
ÂŠ 2019, IRJET
Shear Stress in XY plane
30000000
Stress in Pa
Stress
8.00E+08 6.00E+08 4.00E+08 2.00E+08 0.00E+00 2.00E+08 4.00E+08 6.00E+08 8.00E+08 1.00E+09
Normal Stress in Y direction Shear Stress in XY plane

Impact Factor value: 7.34

No. of divisions of 1 second
Chart 22: Normal stress in X direction and Shear stress in XY plane in Pa for the outer slant edge of the hexagonal cell of t/l ratio 0.005 when a compressive deformation of 0.001 m is applied in the positive and negative X directions.
ISO 9001:2008 Certified Journal

Page 1591
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
The deformation of trends of a regular and a commercial hexagonal cell of t/l ratio 0.005 are also evaluated. Here, only the maximum values of deformation are compared. The following results were obtained when the deformation was observed on the entire cell and on the outer slant edge. The deformation was compressive with a value of 0.001 m in the positive and negative X directions:
Deformation in m X direction Y direction
Regular Hexagonal Cell 3.07E09 8.66E04
Commercial Hexagonal Cell 1.19E08 8.68E04
Regular Hexagonal Cell 6.51E08 3.18E09
Commercial Hexagonal Cell 4.55E08 1.74E08
9. REFERENCES
Table 3: Results for outer slant edge It is observed that when the entire cell is evaluated, the commercial cell has a greater deformation in X direction as compared to the regular cell in the same direction by 4 times, while the deformation in the Y direction remains same. When the outer slant edge is evaluated, it is found that the commercial cell has a greater deformation in X direction by 1.43 times as compared to the regular cell, while the deformation in the Y direction for the commercial cell is greater than the regular cell by a factor of 18.28 times. The following results were obtained when the deformation was observed on the entire cell and on the outer slant edge. The deformation was compressive with a value of 0.001 m in the positive and negative Y directions:
Deformation Regular in m Hexagonal Cell X direction 4.37E04 Y direction 0.001
Regular Hexagonal Cell 2.17E06 0.001
Commercial Hexagonal Cell 9.43E07 1.00E03
When the entire cell is evaluated it is found that the deformation of regular cell is greater than that of the commercial cell in X direction by 1.16 times. But when

Impact Factor value: 7.34
[2]https://en.wikipedia.org/wiki/Honeycomb_conjecture [3] Tom, B., 1997. Honeycomb Technology. Chapman and Hall, London. [4] Hoffman, G.A., 1958. Poisson’s ratio for honeycomb sandwich cores. J. Aerosp. Sci., 25: 534535. [5] Zhao, H. and G. Grrard, 1998. Crushing behavior of aluminum honeycombs under impact loading. Int. J. Impact Eng., 2(10): 827836. [6] Vinson, J.R., 1999. The Behavior of Sandwich Structures of Isotropic and Composite Materials. Technomic Publ., Lancaster PA.
[8] Olympio, K. and F. Gandhi, 2007. Zeroν cellular honeycomb flexible skins for onedimensional wing morphing. Proceeding of the 48th AIAA/ASME/ ASCE/AHS/ASC Structures, Structural Dynamics and Materials sConference. AIAA20071735, Honolulu, Hawaii.
Table 5: Results for outer slant edge
© 2019, IRJET
[1] S. Balawi, J.L. Abot, The effect of honeycomb relative density on its effective inplane elastic moduli: An experimental study, Composite Structures, Volume 84, Issue 4, 2008, Pages 293299, ISSN 02638223.
[7] Khan, M.K., 2006. Compressive and lamination strength of honeycomb sandwich panels with strain energy calculation from ASTM standards. J. Aerospace Eng., 220: 375386.
Commercial Hexagonal Cell 3.75E04 0.001
Table 4: Results for entire cell
Deformation in m X direction Y direction
8. CONCLUSION Hexagonal cells with t/l ratios 0.005 show a much proper trend of deformation as compared to the cell of t/l ratio of 0.3, owing to the characteristic property of cellular solids. The commercial honeycombs also show certain unique deformation trends as compared to the regular hexagonal cells, with the former cell almost always depicting a much higher deformation.
Table 2: Results for entire cell
Deformation in m X direction Y direction
only the outer slant edge is calculated, it is found that the commercial cell has a greater deformation in the X direction as compared to the regular cell by a factor of 2.3 times. The deformation of both regular and commercial cells in Y direction is same when evaluated for the entire cell or the outer slant edge.

[9] Bubert, E., K.S. Woods, C.S. Kothera and N.M. Wereley, 2008. Design and fabrication of a passive 1D morphing aircraft skin. Proceeding of the 49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference. AIAA20082045, Schaumburg, IL. [10] Jaehyung, J., D.S. Joshua, Z. John and F. George, 2010.
ISO 9001:2008 Certified Journal

Page 1592
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
Complaint hexagonal periodic lattice structures having both high shear strength and and high shear strain. J. Mater. Design. [11] Kwangwon Kim, J.J., K. DooMan and Y. HyunSeung, 2012. Modulus and high strain flexure design with auxetic honeycomb structures. IDETC/CIE 2012, DETC201270552. [12] Yanping, L. and H. Hong, 2010. A review on auxetic structures and polymeric materials. Sci. Res. Essays, 5(10): 10521063. [13] Garrard, A., 1949. Theory of sandwich construction II. Br. Plast., 18: 451458.Gaspar, N., X.J. Ren, C.W. Smith, J.N. Grima and K.E. Evans, 2005. Novel honeycombs with auxetic behaviour. Acta. Mater., 53: 24392445. [14] Charles, L. and K.H. Ralph, 1951. Elastic Constants for CorrugatedCore Sandwich Plates. National Advisory Committee for Aeronautics, Washington DC, pp: 105.
reticulated foams: missing rib foam model. Acta. Mater., 48: 43494356. [25] Kwangwon Kim, J.J., K. DooMan and Y. HyunSeung, 2012. Modulus and high strain flexure design with auxetic honeycomb structures. IDETC/CIE 2012, DETC201270552. [26] Jaehyung, J., D.S. Joshua, Z. John and F. George, 2010. Complaint hexagonal periodic lattice structures having both high shear strength and and high shear strain. J. Mater. Design. [27] Gibson, L.J. and F.A. Michael, 1988. Cellular Solids, Structure and Properties. Cambridge University Press, Cambridge. [28] Masters, I.G. and K.E. Evans, 1996. Models for the elastic deformation of honeycombs. Compos. Struct., 35(4): 403422.
[15] Horvay, H., 1952. Bending of honeycombs and of perforated plates. ASME J. Appl. Mech., 19: 122123.
[29] Hohe, J. and W. Becker, 2002. Sandwich cores: Homogenization, material models, and properties. App. Mech. Rev., 55: 6187.
[16] Akasaka, T. and T. Takagishi, 1959. The shear modulus of foil honeycomb sandwich structures. Trans. Japan Soc. Aerospace Sci., 2: 8390.
[30] Balawi, S. and J.L. Abot, 2007b. A reﬁned model for the eﬀective inplane elastic moduli of hexagonal honeycombs. Compos. Struct., 84(2): 147158.
[17] Kelsey, S., R.A. Gellatly and B.W. Clark, 1958. The shear modulus of foil honeycomb cores. Aircraft Eng., 30: 294302.
[31] Balawi, S. and J.L. Abot, 2008. The eﬀect of honeycomb relative density on its eﬀective inplane elastic moduli: An experimental study. Compos. Struct., 84(4): 293299.
[18] Habip, L.M., 1964. A review of recent Russian work on sandwich structures. Int. J. Mech. Sci., 6: 483487.
[32] Patel, M.R. and Finnie, I. (1970) J. Mat., 5,909.
[19] Lui, M. and P. Habip, 1965. A survey of modern developments in the analysis of sandwich structures. Appl. Mech. Rev., 18: 9398. [20] Frostig, Y., 1998. Inaccuracies and validity of simpliﬁed models in the theory of sandwich structures. Proceeding of 4th Int Conference Sandwich Construction. Stockholm, Sweden, Ohlsson, K.A. (Ed.), EMAS Publishing, London, pp: 167189. [21] Theocaris, P.S. and G.E. Panagiotopoulos, 1997. Negative Poisson’s ratio in materials with a starshaped microstructure. A numerical homogenization approach. Arch. Appl. Mech., 67: 274286. [22] Grima, J.N., G. Ruben and P.S. Farrugia, 2008b. The properties of auxetic metatetrachiral structures. Phys. Stat. Sol., 245: 511520. [23] Larsen, U.D., O. Signund and S. Bouwstra, 1997. Design and fabrication of compliant mechanisms and material structures with negative Poisson’s ratio. J. Microelectromech. Syst., 6: 99106. [24] Smith, C.W., J.N. Grima and K.E. Evans, 2000. A novel mechanism for generating auxetic behaviour in
© 2019, IRJET

Impact Factor value: 7.34

[33] Abd ElSayed, F. K. (1976) Ph.D. thesis, Univerity of Sheffield. [34] Abd ElSayed, F. K., Jones, R. and Burgens, I.W. (1979) Composites, 10, 209. [35] Gibson, L. J., Ashby, M. F., Schajer, G. S. and Robertson, C. I. (1982) Proc. R. Soc. Lond., A382, 25. [36] Warren, W. E. and Kraynik, A. M. (1987) Mechanics of Material, 6, 27. [37] Bitzer T. Honeycomb technology. Chapman and Hall: 1997.
10. BIOGRAPHIES SPRIKA GAUR Pursuing Bachelor of Technology in Mechanical Engineering from Govind Ballabh Pant University of Agriculture and Technology, Pantnagar, India.
ISO 9001:2008 Certified Journal

Page 1593
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 06 Issue: 07  July 2019
pISSN: 23950072
www.irjet.net
RASHMI RAMA SUSHIL Completed Bachelor of Technology in Mechanical Engineering from Govind Ballabh Pant University of Agriculture and Technology, Pantnagar, India
Â© 2019, IRJET

Impact Factor value: 7.34

ISO 9001:2008 Certified Journal

Page 1594
https://www.irjet.net/archives/V6/i7/IRJETV6I7520.pdf
Published on Oct 12, 2019
https://www.irjet.net/archives/V6/i7/IRJETV6I7520.pdf